Investigation of fracture toughening mechanisms of asphalt concrete ...

Photo or figure (optional)

**Investigation** **of** **fracture** **toughening**

**mechanisms** **of** **asphalt** **concrete**

using the clustered discrete element method

Hyunwook Kim, Empa, Road Eng./Sealing Components

William G. Buttlar, Univ. **of** Illinois at Urbana Champaign

Manfred N. Partl, Empa, Road Eng./Sealing Components

Conference paper STRC 2008

STRC

8 th Swiss Transport Research Conference

Monte Verità / Ascona, October 15-17, 2008

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

**Investigation** **of** **fracture** **toughening** **mechanisms** **of**

**asphalt** **concrete** using the clustered discrete element

method

Hyunwook Kim

Empa

CH-8600, Dübendorf

Switzerland

Phone: 044-823-4474

Fax: 044-821-6244

email:hyunwook.kim@empa.ch

October 2008

William G. Buttlar

Univ. **of** Illinois at Urbana-

Champaign

61801 Urbana, USA

Phone: 1-217-333-5966

Fax: 1-217-333-1924

email: buttlar@uiuc.edu

I

Manfred N. Partl

Empa

CH-8600, Dübendorf

Switzerland

Phone: 044-823-4113

Fax: 044-821-6244

email:manfred.partl@empa.ch

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

Abstract

Asphalt **concrete** is a quasi-brittle composite material which is composed **of** solid inclusions

and a viscous matrix. The **fracture** **of** heterogeneous solids is a difficult problem to handle

numerically due to the creation and continuous motion **of** new surfaces. A clustered discrete

element method (DEM) is employed as a means to investigate **fracture** **mechanisms** in **asphalt**

**concrete** at low temperatures. A bilinear cohesive s**of**tening model is implemented into the

DEM framework to enable simulation **of** crack initiation and propagation in **asphalt** **concrete**.

The meso-scale representation **of** the morphology **of** the material is incorporated into the

DEM model using high-resolution imaging and image analysis s**of**tware. The bulk properties

and **fracture** parameters **of** multi-phase are obtained from experiments and calibration

procedure. The two-dimensional clustered DEM method is applied into mode I **fracture** tests,

e.g. disk-shaped compact tension (DC(T)) and single-edge notched beam (SE(B)) tests, to

investigate various **fracture** **mechanisms** **of** **asphalt** **concrete**. The simulation results are shown

to compare favourably with experimental results, and moreover, the simulations provide new

insight into the **fracture** **mechanisms** in **asphalt** **concrete**. The modelling technique provides a

physical description **of** the **fracture** process zone in laboratory **fracture** tests and the abilities to

simulate mixed-mode **fracture**, crack competition, and distribution **of** macro- and microcracks.

Keywords

**asphalt** – **fracture** - discrete element method - cohesive s**of**tening model –DC(T) – SE(B)

II

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

1. Introduction

The fracturing **of** **asphalt** **concrete** paving surfaces and overlays is a significant cause **of**

premature pavement deterioration. Cracks at the pavement surface create a permanent

maintenance liability, and those which extend through the thickness **of** pavement reduce

structural capacity and greatly increase pavement permeability and the intrusion **of** moisture

into the pavement foundation. Asphalt **concrete** is a quasi-brittle composite material which is

composed **of** solid inclusions (aggregates) and a viscous matrix (**asphalt** mastic). The mastic

is composed **of** fine aggregates and **asphalt** binder and is the “glue” material holding larger

aggregates together. The **fracture** **of** heterogeneous solids is a difficult problem to handle

numerically due to the creation and continuous motion **of** new surfaces. The use **of** linear

elastic **fracture** mechanics (LEFM) to analytically describe these **mechanisms** would be

approximate, since the **fracture** patterns typically consist **of** a main crack, crack branching,

secondary cracks, and microcracks.

However, there has been very limited work directed towards the development and/or

application **of** models that can simulate the propagation **of** cracks in **asphalt** pavements while

adequately considering the material’s distinctive heterogeneity. Without the ability to model

crack movement, it is not possible to properly assess crack initiation and the complexity **of**

crack propagation. Typically, three general approaches can be employed in a research

investigation, namely: experimental observations, analytical modeling, and numerical

modeling. Experimental measurements can provide material properties and descriptions **of**

material behavior, but the results may be affected by the boundary conditions, such as

specimen size, geometry, and characteristics **of** the testing device. Analytical models can

provide ‘exact’ answers and useful benchmark solutions, but are limited to relatively simple

boundary value problems with highly idealized and simplified material properties. Numerical

methods can be employed to extend analytical methods to consider more complex boundary

conditions and material constitutive models, as has been demonstrated with the finite element

method over the past several decades. However, modern numerical analysis techniques have

the added advantage **of** allowing the study **of** the interaction between microstructural material

properties and specimen geometry. For instance, information about the material structure at

the meso-level can be incorporated into the numerical model, as shown in Figure 1.

3

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

Figure 1 Model calibration procedure with experimental and numerical methods

The main objective **of** this study is the initial step **of** a long-term project to investigate

micromechanical **fracture** **mechanisms** in **asphalt** **concrete** using clustered discrete element

method in conjunction with a high-resolution image technique. The long-term goal is the

accurate prediction **of** laboratory and pavement **fracture** **mechanisms** and the development **of**

design method to consider the **fracture** **mechanisms** **of** **asphalt** materials. However, due to

time limitations, the integration **of** laboratory testing and numerical modeling is the focus **of**

this study. The approach used herein incorporates experimental testing, multi-scale numerical

simulation, image processing, and field performance. The micromechanical **fracture**

modeling approach used can be viewed as an early developmental step towards the “virtual

**asphalt** laboratory”, where simulations **of** laboratory tests and eventually field response and

distress predictions can be made to enhance our understanding **of** pavement distress

**mechanisms**, such as thermal **fracture** or reflective cracking. The DEM will ultimately be

used in multi-scale modeling, where global pavement response and local **fracture** behavior can

be considered in the same numerical simulation.

4

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

2. Constitutive laws

2.1 Discrete element method

The discrete element method (DEM) originally developed by Cundall (1971) has proven to be

a power and versatile numerical tool for modeling the behavior **of** granular and particulate

systems, and also for studying the micromechanics **of** materials such as soil at the particle

level. Also, the method has the potential to be an effective tool to model continuum

problems, especially those that are characterized by a transformation from a continuum to

discontinuum. The DEM discretizes a material using rigid elements **of** simple shape that

interact with neighboring elements according to interaction laws that are applied at points **of**

contact.

The analysis procedure consists **of** three major computational steps: internal force evaluation,

in which contact forces are calculated; integration **of** equations **of** motion, in which element

displacement are computed; and contact detection, where new contacts are identified and

broken contacts are removed. In a DEM analysis, the interaction **of** the elements is treated as

a dynamic process that alternates between the application **of** Newton’s second law and the

evaluation **of** a force-displacement law at the contacts. Newton’s second law gives the

acceleration **of** an element resulting from the force acting on it, including gravitational forces,

external forces prescribed by boundary conditions, and internal forces developed at interelement

contacts. The acceleration is then integrated to obtain the velocity and displacement.

The force-displacement law is used to find contact forces from known displacement. The

equations **of** motion are integrated in time using the central difference method. The method

can be computationally very demanding and thus, efficient algorithms, especially for the

internal force evaluations and contact detection, must be used. Computational effectiveness

will be particularly important for three-dimensional discretizations, the use **of** which is

inevitable for obtaining fully realistic and accurate models for many applications. In the

absence **of** damping, the DEM equilibrium equation at discrete time intervals for the system

**of** particles is following:

Error! Objects cannot be created from editing field codes.

Where, M is the mass matrix, a is the acceleration vector, K is the stiffness matrix, Δf is the

incremental force vector, and Δx is the incremental displacement vector.

5

(1)

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

The translational and rotational stiffnesses **of** a particle relate increments **of** force and moment

to increments **of** displacement and rotation via the matrix relations:

Error! Objects cannot be created from editing field codes.

In a two-dimensional system, equation (2) can be expressed as:

Error! Objects cannot be created from editing field codes.

The individual elements **of** this stiffness matrix can be expressed for a particular contact in

terms **of** the particle radius r, the contact normal vector ni, and the contact stiffnesses, i.e. K n

and K s . Again, equation (2) can be expressed with the terms in a standard FE frame work

from equation (4) to equation (7):

Error! Objects cannot be created from editing field codes. (4)

Error! Objects cannot be created from editing field codes.

Error! Objects cannot be created from editing field codes. (6)

Error! Objects cannot be created from editing field codes.

Where, {Δf} are the incremental force vectors, [K] is the contact stiffness matrix, {δu} are the

contact displacements, {ε} are the contact strains, {σ} are the contact stresses, [B] is the strain

matrix and [D] is the elasticity matrix.

The elements **of** the stiffness matrix represent primarily the normal and shear springs that are

present at the contact points. The stiffness matrix ([K]) changes during the analysis as

contacts are formed and broken. Discrete element simulations can therefore be classified as

non-linear, dynamic analyses. The principal difference between the available DEMs is the

time integration algorithm used to solve equation (1) (O’Sullivan and Bray, 2001). Equation

(2) is similar to the global equation considered in continuum finite element modeling.

6

(2)

(3)

(5)

(7)

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

The constitutive models used in the current two-dimensional (2-D) clustered DEM application

consist **of** three parts: a contact stiffness model, a slip friction model and a bonding model.

The linear contact model is defined by the normal and shear stiffness kn and ks

(force/displacement) **of** the two contacting entities (ball-to-ball or ball-to-wall) acting in

series. The contact normal secant and shear tangent stiffness are given by:

Normal secant stiffness:

Error! Objects cannot be created from editing field codes.

Shear tangent stiffness:

Error! Objects cannot be created from editing field codes.

The normal stiffness is a secant stiffness and it linearly relates the total normal force to the

total normal displacement.

Error! Objects cannot be created from editing field codes.

(10)

The shear stiffness is a tangent stiffness and it relates the increment **of** shear force to the

increment **of** shear displacement.

Error! Objects cannot be created from editing field codes.

(11)

The slip friction model is an intrinsic property **of** the two entities in contact (ball-to-ball or

ball-to-wall) that governs frictional sliding **of** unbonded or debonded particles (ITASCA,

2002). The slip and bond models describe the constitutive behavior governing the response **of**

particle contact points. The slip model is defined by the friction coefficient at the contact.

For bonded assemblies, if the applied force becomes larger than the maximum allowable

shear contact force, then slip is allowed to occur. The bond model allows particles to be

joined at contacts, which activates material stiffness in opening and shear. The constitutive

behavior for contact occurring at a point for the normal and shear components are given by

Figure 2(a). S n and S s are normal and shear bond strengths; F r is the frictional force. Figure

2(b) illustrates the calculation cycle. At the start **of** each time step, the set **of** contacts is

7

(8)

(9)

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

updated from the known particle and wall positions. The force-displacement law is then

applied to each contact to update the contact forces based on the relative motion between the

two entities at the contact and the contact constitutive model. Next, the law **of** motion is

applied to each particle to update its velocity and position based on the resultant force and

moment arising from the contact forces and any body forces acting on the particle. Also, the

wall positions are updated based on the specified wall velocities.

Figure 2 Constitutive models and calculation cycle

(a) Constitutive Contact, Slip, and Bond Model

Applied Force

Particles Contacts

Law **of** Motion

Hooke’s Law

(F=ma)

(F=kx)

- Particles: Resultant Force + Moment

- Contacts: Relative Motion,

Constitutive Law

2.2 Cohesive s**of**tening model

8

• Update:

-Particles

- Wall Positions

- Set **of** Contacts

-Contact Force

(b) Calculation Cycle **of** Discrete Element Method

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

Dugdale (1960) and Barenblatt (1962) proposed cohesive models to investigate ductile and

brittle material **fracture** behavior, respectively. The cohesive crack concept was later

successfully extended by Hillerborg et al. (1976) to study nonlinear **fracture** processes in

Portland cement **concrete**. Furthermore, cohesive zone models (CZMs) have been used to

simulate the **fracture** process in a number **of** material systems under a variety **of** loading

conditions (static, dynamic, cyclic, etc). The two most noteworthy cohesive failure models

available in the literature are: the intrinsic potential-based model and extrinsic linear law

model. In the intrinsic approach, the failure criterion is incorporated within the constitutive

model **of** the cohesive elements. Failure is integrated into the cohesive law by increasing the

cohesive tractions from zero to a failure point at which the tractions reach a maximum before

gradually decreasing back to zero. In all intrinsic CZMs, the traction-separation relations for

interfaces are such that with increasing interfacial separation, the traction across the interface

reaches a maximum, then decreases and eventually vanishes, permitting a complete

decohesion. The main difference between CZMs lies in the shape **of** the tractiondisplacement

response. Bilinear CZMs can be described by two independent parameters.

These parameters may be two **of** the three parameters, namely the cohesive energy Φ, and

either **of** the cohesive strength σmax, or the separation/critical length δsep.

Figure 3 Schematic concept **of** bilinear cohesive s**of**tening model

9

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

An intrinsic general cohesive s**of**tening model (CSM) is implemented as a user-defined model

in the particle flow code (PFC-2D), which is in the form **of** a bilinear cohesive zone model

(Figure 3(c)). In general, the cracking **of** **asphalt** **concrete** can occur in any weak point within

the **fracture** process zone (Figure 3(a)) and the cohesive **fracture** concept at the crack tip can

be simplified as shown in Figure 3(b). Geubelle et al. (1998) utilized a bilinear CZM to

simulate spontaneous initiation and propagation **of** transverse matrix crack and delaminating

fronts in thin composite plates subjected to low-velocity impact. In Figure 3(c), δmax

represents the location **of** cohesive crack tip and δsep is the complete material separation or the

material crack tip, and σmax is the normal cohesive strength. Point B represents the starting

point **of** unrecoverable material degradation (or micro-crack initiation) and point C represents

the condition where a crack face has fully separated and has released the energy potential

associated with decohesion.

If the contact is in tension, the contact strength Fmax is calculated from the two strength

parameters (i.e. normal force, F n c and shear force, F s c) as a function **of** the current orientation

**of** the contact force. It is assumed that contact strength varies as a linear function **of** the

angleα :

2α

n 2α

F max = ( 1−

) × Fc

+ × F

π π

Where, α is the angle between the directions **of** contact force and the line segment connecting

the centers **of** particles. The yielding **of** bond in tension is determined by comparing the

resultant contact force, i.e., with the contact strength.

n 2

F = ( F ) +

The contact yields if the contact force is larger than the contact strength. In the present

**fracture** modeling approach, Mode I (i.e., pure opening) **fracture** behaviors are dominant in

both homogenous and heterogeneous specimen **fracture** simulations. However, unlike the

homogenous mode I simulation where shear separations are negligible, in the heterogeneous

material simulation, the meandering cracking activates a non-negligible amount **of** mixedmode

interface behavior (crack opening and sliding).

In the case **of** yielding **of** contact bonds, the increment **of** contact displacements, ΔU k (k=n, s),

can be decomposed into elastic and plastic contact displacement increments:

10

( F

s

)

2

s

c

(12)

(13)

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

Δ

k k

U = ΔU

e + Δ

The force increment, ΔF k , is a function **of** incremental elastic displacement only:

Where,

Δ

Δ

k k

F = K Δ

U

11

k

e

k k

U e = ΔU

− Δ

The elastic (or plastic) displacement increment can be determined using the consistency

condition (i.e., F - Fmax = 0). In the s**of**tening portion **of** the model, the contact strength is a

function **of** the accumulated plastic deformation, as described by:

Where,

U

U

k

p

U

k

k

Fc ( U p / U p max ) = Fc

( 1−

U

U

p

∑ ΔU

= p

k

p

p

p max

)

(14)

(15)

(16)

(17)

(18)

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

3. Experimental tests

3.1 Single-edge notched beam test

Figure 4 llustrates a simply-supported, single-edged notched beam (SE(B)) with a length **of**

376 mm, a height **of** 100 mm and a thickness **of** 75 mm. A notch was then inserted with a

length **of** 19 mm, giving a notch to depth (a/H) ratio **of** 0.19. The depth **of** the notch was

selected to be long enough to ensure adequate stress intensity at the notch tip to initiate a

crack, but short enough to ensure a ligament **of** adequate length for test repeatability and to

prevent crack initiation under self-weight. The constant crack mouth opening displacement

(CMOD) loading rate, 0.7 mm/min, is imposed at the center **of** the top edge **of** the specimen

in order to predict stable **fracture** behavior. As shown in Figure 4, a clip-on gauge with a

range **of** 6.35 mm was used for measuring the CMOD. The CMOD gage was attached to the

beam using gage points that were glued to the edge **of** the notch. The test was conducted in a

temperature controlled environmental chamber capable **of** maintaining air temperature within

±0.2 °C.

Figure 4 SE(B) geometry and test configuration

(a) SE(B) Test Geometry

12

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

(b) Test Configuration and Clip-on Gage

3.2 Disk-shaped compact tension test

The main purpose for the development **of** the disk-shaped compact tension (DC(T)) test

specimen geometry was the ability to test cylindrical cores obtained from in-place **asphalt**

**concrete** pavements and gyratory-compacted specimens fabricated during the **asphalt** **concrete**

mixture design process for relevant **fracture** properties. The dimensions **of** the specimen were

determined by using the ASTM E399 Standard as a guideline. As shown in Figure 5(a) and

Table 1, the specimen diameter is 150mm and both cored hole diameters within the specimen

are 25mm. The width **of** the specimen (W) was 110 mm with the notch length (a) being 27.5

mm (a/W = 0.25). Therefore, the initial ligament length (W-a) was 82.5 mm. The thickness

(t) **of** the specimen was 50 mm. The dimensions noted in the figure were initially developed

for 9.5 mm NMAS mixtures, but has been successfully applied to 4.75 mm and 19 mm

NMAS mixtures. Figure 5(b) shows DC(T) test configuration and clip-on gage. The DC(T)

test is loaded in tension through the loading holes and is conducted with a constant CMOD

rate **of** 1 mm/min.

13

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

Figure 5 DC (T) Specimen Geometry for Asphalt Concrete

(a) DC (T) Specimen Geometry (b) DC(T) Test Configuration and Clip-on Gage

Table 1 DC(T) Dimension

Dimension mm

D 150

W 110

a 27.5

d 25

C 35

Φ 25

t 50

14

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

4. Material properties and image analysis

Two different mixtures (LR-19 and LR-9.5) were used with the same aggregate type

(dolomite limestone) from a local central Illinois source in USA. The materials used herein

are **asphalt** mixtures with 9.5mm and 19mm nominal maximum aggregate size (NMAS). The

aggregate gradation plot is shown in Figure 6. PG64-22 binder was used for both mixtures.

Figure 6 Aggregate gradations **of** **asphalt** mixtures with 9.5 mm NMAS

One **of** the important procedures to make a heterogeneous **fracture** model is the image

processing to capture the real microstructure using high-resolution image scanning

(Resolution: 1600×1600, Pixel size: 0.016 mm) and user-defined program, which can detect

aggregate locations and shapes in **asphalt** mixtures. As illustrated in Figure 7 and Figure 8, a

digital image can be obtained from the specimen via scanning and projected onto a discrete

element mesh using Image-Pro Plus (Media Cybernetics, 2004) and a user-defined Excel

VBA program. Next, the holes which facilitate loading pins and the mechanical notch are

simulated by removing appropriate elements in the simulated specimen. DC(T) DEM

specimens which capture the sand-size (0.3 mm) and larger aggregate features **of** 19mm

nominal maximum aggregate size (NMAS) mixtures can be obtained with this technique.

Also, some **of** important information such as each aggregate area, aspect ratio, diameter and

perimeter, aggregate angle, and roundness can be obtained and analyzed to investigate the

sensitivity **of** microstructure on the **fracture** process.

15

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

Figure 7 Image projection procedure **of** microstructure into DEM mesh

Figure 8 Numerical and laboratory DC(T) specimen images

16

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

(a) DEM Specimen Representation (Left) and Laboratory Specimen (Right)

Mastic

Aggregate

(b) DEM mesh around a notched crack tip

Figure 9 schematically illustrates modeling approaches used for the heterogeneous cohesive

**fracture** investigation using PFC-2D. The **asphalt** **concrete** specimen was divided into three

phases: aggregate, mastic, and interface between aggregate and mastic. For the material

**fracture** properties, it was assumed that each phase has a material **fracture** behavior such as

linear elastic for aggregate, bilinear elasto-plastic for mastic, and bilinear elasto-plastic for

interface because **of** the s**of**tening **of** one side mastic. But the s**of**tening displacement **of**

interface is much smaller than that **of** mastic (Ince et al., 2003). As illustrated in Figure 9,

each phase requires an independent set **of** material parameters namely: Young’s modulus;

tensile strength, and **fracture** energy. Current experimental procedures limit the ability to

measure all **of** the required parameters, especially the interface parameters. A limited number

**of** experiments conducted on the aggregates, mastics, and mixtures, combined with typical

values obtained in the literature (Tschegg et al., 1995) allowed for the determination **of** most

material parameters (i.e., Young’s modulus, tensile strength, and **fracture** energy for both

aggregate and mastic). For the remaining parameters (i.e., tensile strength and **fracture** energy

for the interface between aggregate and mastic), calibration procedure was used to estimate

from assumed seed values. A sensitivity analysis was conducted to determine the effect **of** the

interfacial properties on the global **fracture** response. The goal **of** the sensitivity analysis was

not necessarily to match experimental results but rather to develop the understanding **of** the

effects **of** the interfacial properties. The details **of** sensitive analyses are beyond the scope **of**

this paper but can be found in author’s publications (Kim et al., 2008(a)).

17

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

Figure 9 Multi-phase DEM geometries and assumed material properties

DC(T) Microstructure

Aggregate Aggregate Aggregate

Mastic

Interface Interface Interface

18

σσ

σ

Linear Elastic Contact

σσ

σ

δδ

δ

δδ

δ

Bilinear Cohesive Contact

σσ

σ

δδ

δ

Bilinear Adhesive Contact

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

5. Numerical results

5.1 Heterogeneous SE(B) modeling

Figure 10 represents the numerical heterogeneous model geometry and crack propagation

results. In this model, 149,922 particles with 0.25mm radius and 298,855 contacts are used

across the entire specimen and 61,717 particles and 105,236 contacts are used to model

aggregates; 88,205 particles and 158,042 contacts for mastic, and; 35,577 contacts are used at

the interfaces between aggregate and mastic sub-particles (Kim et al., 2008(b)). The material

parameters **of** aggregate and mastic were obtained from indirect tension (IDT) and dynamic

modulus tests (You, 2004). The material parameters **of** interface were assumed that they are

similar to the mastic. The **fracture** energies **of** mastic and interface were estimated and

calibrated based on the experimental **fracture** test data **of** mixture. The stress concentration in

the ligament along the expected mode I crack path is significant and many micro-cracks were

predicted in the process zone prior to crack propagation, as shown in Figure 10. Figure 10(b)

show many micro-cracks around an aggregate in the top **of** notched crack tip. From the

experimental tests and numerical simulations, the powerful potential benefits **of** DEM **fracture**

model can be discussed. The **fracture** **of** **asphalt** **concrete** has very different **fracture**

**mechanisms** due to the non-homogeneity in the specimen such as micro-cracking, crack

branching and deflection, crack face sliding, crack bridging, and crack tip blunting. The

micro-cracking phenomenon consumes a part **of** the external energy caused by the applied

load. Crack deflection occurs when the path **of** least resistance is around a relatively strong

particle or along a weak interface. Also, during the opening **of** a tortuous crack, there must be

some frictional sliding between the cracked faces that causes energy dissipation through

friction. Based on these **mechanisms** in the **fracture** **of** **asphalt** **concrete**, heterogeneous DEM

**fracture** model can have the ability to gain some insight towards **fracture** **toughening**

**mechanisms** in **asphalt** **concrete**.

19

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

Figure 10 Heterogeneous DEM **fracture** model and representations **of** cracks

For the calibrated heterogeneous **fracture** simulation, the overall trend resembled the

experimental result as shown in Figure 11. Due to the presence **of** a large aggregate just

ahead **of** the simulated notch, the force was predicted to experience a sudden decrease before

the peak load but then was recovered. This phenomenon has been observed in experimental

trials, particularly when thin specimens with larger aggregates are tested. Thus, the 2D

model herein tends to exaggerate the effect **of** aggregates on the load-CMOD response,

especially when compared to experimental results obtained from specimens with larger

thicknesses-to-maximum-aggregate size ratios. Thus, the need for three-dimensional

modeling to accurately capture material heterogeneity is apparent.

20

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

Figure 11 Experimental and numerical responses (9.5mm NMAS at -10 °C)

The mixed-mode **fracture** in a pavement system is popular and significant due to the presence

**of** continuous dynamic and static traffic loads and environmental conditions including

temperature and moisture. Using the calibrated cohesive parameters and particle size

0.25mm, the mixed-mode problem was investigated herein using the SE(B) test with an **of**fset

notch to create mixed-mode (i.e., mixed with Mode-I and Mode-II) crack propagation. The

shear parameters **of** **fracture** properties were the same with normal parameters. The **of**fset

parameters, γ, as defined in Figure12, were 0.4, 0.5, and 0.55 resulting in **of**fset lengths **of** 65

mm, 81 mm, and 89 mm from the middle **of** specimen.

Figure 12 Mixed-mode SE(B) geometry with **of**fset notch

21

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

Figure 13 shows the crack paths for the three beams, plus the standard SE(B) beam (γ = 0).

Based on the test results, the critical **of**fset was between γ =0.5 and 0.55. Although only one

material was tested, the critical **of**fset should depend on the material toughness and also on the

notch depth. Therefore, the study should be extended to investigate different materials and

notch lengths to provide a full experimental investigation. Figure 13(b) shows the numerical

failed beams with 0.55 notch **of**fset and the crack propagation was progressed from the middle

**of** the specimen.

Figure 13 Experimental and numerical trajectories path with various notch **of**fsets

γ = 0.0

γ = 0.4

γ = 0.5

γ = 0.55

22

Front

Back

Centerline

(a) Experimental crack trajectories

S

γ∗S/2

(b) Numerical crack trajectories (γ = 0.55)

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

For the beam with 0.4 notch **of**fset, the macro-crack initiated with mode-I fracturing in but the

path quickly began to meander at an angle towards the loading point as the crack propagated.

Before crack initiation, inelastic effects at the crack tip in the notched region and in the

vicinity **of** the outer fiber **of** bending at the bottom **of** the mid-span **of** specimen are

simultaneously occurring (Figure 14).

Figure 14 Progressive crack initiation and propagation by numerical model (γ = 0.4)

(a) Micro-Crack Initiation (b) Macro-Crack Initiation (c) Crack Propagation

5.2 Heterogeneous DC(T) modeling

Heterogeneous DC(T) **fracture** simulations were done to verify the SE(B) results if the

predicted material parameters could be fitted into different test modes. The heterogeneous

cohesive **fracture** simulation **of** a 19mm NMAS mixture was comprised **of** a total **of** 38,721

discrete elements, each having 0.35mm radius forming 114,994 contacts in the horizontal

hexagonal packing arrangement. For the clustered DEM technique used in this study, the

microstructure was mapped upon a uniformly generated sheet **of** hexagonally arranged

circular elements. The diameter **of** the discrete element was carefully selected so that

irregular geometrical features, such as aggregates, can be modeled by bonding a number **of**

elements together and assigning the proper material properties within the bonded clusters and

at the interface between aggregates and mastic. Various **fracture** mechanism related to

temperature and microstructure could be investigated by heterogeneous DEM **fracture** models

(Kim and Buttlar, 2005).

23

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

Figure 15 Comparisons **of** experimental and numerical results at different temperatures

(a) Force vs. CMOD Curves at Different Temperatures

(b) Crack Trajectory at -10 °C (c) Crack Trajectory at 0 °C

Table 2 Heterogeneous DEM model parameters at different temperatures

9.5 mm NMAS Material Properties DEM Contact Properties

Temperature

(°C)

Phase

Young’s

Modulus

(GPa)

24

Tensile

Strength

(MPa)

Stiffness

(GPa)

Bond Strength

(MPa)

-10°C (B: 54mm) Aggregate 56.8 6.59 2.9 169

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

0°C (B: 51mm)

Mastic 14.2 3.0 0.77 82

Interface 14.2 2.8 0.77 74

Aggregate 56.8 6.59 2.9 169

Mastic 9.9 2.7 0.51 69

Interface 9.9 2.5 0.51 63

Using more successful aforementioned image analysis, numerical simulations with the same

microstructure as experimental specimens were compared. Figure 16 and Figure 17 compare

the experimental and numerical results including crack path and trajectories, force vs. CMOD

curves, micro-cracks, and stress concentration in the **fracture** process zone area. The microcracking

**of** the DEM model occurred when the s**of**tening starts in the local model after

passing the material strength.

Figure 16 Crack trajectories and force vs. CMOD curves (19mm NMAS)

(a) A Comparison **of** Crack Trajectories and Micro-Cracks

25

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

(b) Comparisons **of** Experimental and Numerical Results

Figure 17 Crack trajectories and force vs. CMOD curves (9.5mm NMAS)

(a) A Comparison **of** Crack Trajectories and Stress Concentration

26

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

(b) Comparisons **of** Experimental and Numerical Results

An important finding from this exercise is that complete material separation just ahead **of** the

mechanical notch in the 150 mm diameter DC(T) specimen occurs only after peak load is

reached in the experiment. This suggests that the **fracture** process zone (FPZ) is relatively

large as compared to specimen dimensions, suggesting that linear elastic **fracture** mechanics

principles should not be expected to hold for HMA. The FPZ is a nonlinear zone

characterized by progressive s**of**tening, where the traction across the forming crack surface

decreases as separation increases. The different **fracture** **toughening** **mechanisms** **of** brittle,

quasi-brittle, and ductile materials are greatly influenced by the characteristics **of** the FPZ.

Since the FPZ consumes a substantial amount **of** the energy supplied by the applied load, the

presence **of** the **fracture** process zone is important for the **fracture** response after the peak load

is reached. To study this phenomenon in more detail, the extent **of** the zones **of** compression,

tension, s**of**tening and **fracture** in the DC(T) specimen as a function **of** CMOD (and thus time)

were obtained from the DEM simulations. As shown in Figure 18, the extent **of** the s**of**tening

zone increased until well after crack initiation and then gradually decreased as the crack

propagated. Clearly, the s**of**tening zone size is affected by proximity to the specimen

boundary, due mainly to the flexure present in the DC(T) test, not unlike that present in

bending tests. Once again, the size **of** the **fracture** process zone is far from negligible, since at

times during the test it encompasses more than half **of** the eventual **fracture** ligament.

27

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

Figure 18 Numerical progressive **fracture** process (19mm NMAS at -10 °C)

28

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

6. Conclusions and discussions

A micromechanical **fracture** modeling approach has been employed to investigate various

**toughening** mechanism in the **fracture** **of** **asphalt** **concrete**. Using a high-resolution image

technique, the microstructure **of** **asphalt** mixture was obtained and directly considered in the

**fracture** modeling approach. Mode-I and mixed-mode **fracture** models were implemented,

simulated, and compared with experimental (DC(T) and SE(B)) test data to validate the

numerical results and to determine the material parameters using calibration procedure.

Numerical results matched well with experimental results, even in cases where different test

modes were simulated using the same multi-phase material parameters.

The heterogeneous **fracture** simulation demonstrated the potential usefulness **of** the approach

in the investigation **of** **fracture** **mechanisms** in **asphalt** **concrete**. A near-term application **of**

the discrete element modeling techniques presented is the ability to simulate several

laboratory tests, such as creep, stiffness, strength, and **fracture**, with essentially the same

material ‘fabric’. The simulation **of** numerous laboratory tests can be used to reduce the

amount **of** expensive and time-consuming experimental tests required for mechanisticempirical

design and analysis programs. Some **of** works related to the specimen size

dependency and the rate-dependent **fracture** behavior were already done and have been

continuously investigating (Kim et al., 2009(a) and Kim et el., 2009(b)). Future work in areas

such as three-dimensional (3-D) image analysis using the x-ray tomography (Partl et al.,

2003), 3-D heterogeneous modeling; large-scale, e.g. pavement system modeling;

experimental determination **of** interface material properties; systematic or statistical modeling

**of** material defects and air voids; dynamic **fracture** modeling will lead to even more powerful

modeling capabilities.

29

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

7. References

Barenblatt, G.I. (1962) Mathematical theory **of** equilibrium cracks in brittle **fracture**,

Advances in Applied Mechanics, Vol. 7, pp. 55-129.

Cundall, P. A. (1971) A computer model for simulating progressive, large-scale movements

in blocky rock systems, Proceedings **of** the International Symposium **of** Rock Fracture,

Nancy, France, paper no. II-8.

Dugdale, D. (1960) Yielding **of** steel sheets containing slits, Journal **of** Mechanics and

Physics **of** Solids, Vol. 8, pp. 100-104.

Geubelle, P. H. and J.S. Baylor (1998) Impact-induced delamination **of** composites: a 2D

simulation”, Composites Part B, 29B, 589-602.

Hillerborg, A., M. Modeer, and P.E. Petersson (1976) Analysis **of** crack formation and crack

growth in **concrete** by means **of** **fracture** mechanics and finite elements, Cement and

Concrete Research, Vol. 6, No. 6, pp. 773-782, Nov.

Ince, R., A. Arslan, and B.L. Karihaloo (2003) Lattice modeling **of** size effect in **concrete**

strength, Engineering Fracture Mechanics, Vol. 70, 2307-2320.

ITASCA Consulting Group, Inc. (2002) PFC 2D version 3.0, Minneapolis, Minnesota 55415,

USA.

Kim, H. and W.G. Buttlar (2005) Micromechanical **fracture** modeling **of** hot-mix **asphalt**

**concrete** based on a disk-shaped compact tension test”, Journal **of** the Association **of**

Asphalt Paving Technologists, Volume 74E.

Kim, H., M.P. Wagoner, and W.G. Buttlar (2008(a)) Simulation **of** heterogeneous cohesive

**fracture** model in **asphalt** **concrete** using discrete element method, Journal **of** Materials

in Civil Engineering, Vol. 20, No. 8, pp.552-563.

Kim, H., M.P. Wagoner, and W.G. Buttlar (2008(b)) Experimental and numerical prediction

**of** **fracture** behavior **of** **asphalt** mixture using single-edge notched beam test, Materials

and Structures, (In press).

Kim, H., M. P. Wagoner, and W.G. Buttlar (2009(a)) Numerical **fracture** analysis on the

specimen size dependency **of** **asphalt** **concrete** using a cohesive s**of**tening model,

Construction and Building Materials, (In press).

Kim, H., M.P. Wagoner, and W.G. Buttlar (2009(b)) Rate-dependent **fracture** modeling **of**

**asphalt** **concrete** using the discrete element method, Canadian Journal **of** Civil

Engineering, (In press).

Partl, M.N., A. Flisch, and M. Jönsson (2003) Gyratory compaction analysis with computer

tomography, Road Materials and Pavement Design, Vol.4(4), pp.401-422.

30

8 th Swiss Transport Research Conference

_____________________________________________________________________________ October 15-17, 2008

Media Cybernetics Inc. (2004) Image-Pro Plus 5.0, Silver Spring, Maryland, USA.

O’Sullivan, C. and J.D. Bray (2001) A comparative evaluation **of** two approaches to discrete

element modeling **of** particulate media, Proceedings **of** the Fourth International

Conference on Discontinuous Deformation, pp.97-100, University **of** Glasgow,

Scotland, UK.

Tschegg, E.K., H.M. Rotter, P.E. Roelfstra, U. Bourgund, and P. Jussel (1995) Fracture

mechanical behavior **of** aggregate – cement matrix interfaces, Journal **of** Materials in

Civil Engineering, Vol. 9, No. 4, pp.199-203.

You, Z. and W.G. Buttlar (2005) Discrete element modeling to predict the modulus **of** **asphalt**

**concrete** mixtures, ASCE Journal **of** Materials in Civil Engineering, Vol. 17, pp. 140-

146.

31